eco-dyeing of nylon fabric using natural dyes extracted ... protein fibers such as wool and silk dye
Post on 30-Oct-2019
Embed Size (px)
International Journal of Scientific & Engineering Research, Volume 7, Issue 9, September-2016 1030 ISSN 2229-5518
IJSER © 2016 http://www.ijser.org
Eco-dyeing of Nylon Fabric Using Natural Dyes Extracted from Onion Outer Shells:
Assessment of the Effect of Different Mordant on Color and Fastness
Properties. Mohammad Raza MIAH1, Zakaria2, Md Adnan Hossain3, Atharul Islam Dipto4, Felix Y Telegin 5, Heng Quan6
1,2,5,6School of Chemistry and Chemical Engineering, Wuhan Textile University, Fang Zhi Road 1, Wuhan, 430073, P.R. China.
1,6Color Root (Hubei) Technology Co., Ltd, No.1, Liyuan Avenue, Chendian Town, Songzi City, Hubei, China.
1 Department of Textile Engineering, Bangladesh University of Business and Technology, Dhaka Commerce College Road, Mirpur-2, Dhaka-1216, Bangladesh.
3,4 School of Management, Wuhan Textile University, Fang Zhi Road 1, Wuhan, 430073, P.R. China. 2,4Department ofKnitwear Manufacture and Technology, BGMEA University of Fashion & Technology
(BUFT), SR Tower, 105 Uttara Model Town, Sector-7, Dhaka-1230, Bangladesh. 3Department of Apparel Manufacture and Technology, BGMEA University of Fashion & Technology
(BUFT), SR Tower, 105 Uttara Model Town, Sector-7, Dhaka-1230, Bangladesh. 5Department of Organic Chemistry, Ivanovo State University of Chemistry and Technology, Engels Ave 7,
Ivanovo, 153000, Russia.
1email: firstname.lastname@example.org , 2email: email@example.com, 3email: firstname.lastname@example.org , 4email: email@example.com , 5email: firstname.lastname@example.org , 6email: email@example.com
Abstract: Onion (allium cepa) extract has been used in textile and leather industry as a colorant. Natural colors have attracted the attention of the entire world because of their non-hazardous nature. In the present study, nylon fabric was dyed with onion (allium cepa) natural dye using various mordants such as alum, copper sulphate and potassium dichromate by HTHP dyeing methods. The dyeing behavior of dyes was assessed by colorimetric evaluations of fabrics were carried out by spectrophotometer. Good wash-fastness, rubbing-fastness, light-fastness, water-fastness and perspiration-fastnesswere obtained.
Keywords: Onion (Allium cepa) natural dye, HTHP, Mordant, Nylon fabric.
1 Introduction Recently environmental concerns have created an increasing demand for natural dyes which are friendlier to the environment than synthetic dyes. Synthetic dyes have a wide range of hazardous effect. They are toxic or poisonous, corrosive (destructive to living tissues), irritants (induce local inflammatory reaction in living tissues), infection (represent a potential source of the transmission of diseases to human, domestic animal or wild life), radioactive etc. Natural dyes are non-carcinogenic, produce soothing and exclusive color to the textiles, and have better biodegradability and higher compatibility with the
http://www.ijser.org/ mailto:firstname.lastname@example.org mailto:email@example.com mailto:firstname.lastname@example.org mailto:email@example.com mailto:firstname.lastname@example.org mailto:email@example.com
International Journal of Scientific & Engineering Research, Volume 7, Issue 9, September-2016 1031 ISSN 2229-5518
IJSER © 2016 http://www.ijser.org
environment. Among the natural dyes, plant dyes are potential sources because of their easy availability and abundant nature. Natural dyes have many advantages, such as low toxicity and allergic reactions in addition to bio-degradability because they are taken from animal or plant matter without chemical processing. However, the use of natural dyes declined to a great extent with the advent of synthetic dyes, which have moderate-to-excellent color fastness properties in 1865. During the decade of the 1990s, the textile and apparel industries, particularly the coloration industry, have been widely criticized for their role in polluting the environment. For these reasons, the use of carcinogenic dyes has been restricted and the use of natural dyes has increased [1,2,3,4,5,6,7,8,9,10].The use of synthetic dyestuffs during their application in the dyeing and printing industries has been criticized due to introduction of contaminants into the environment. This has led to the desire to turn to the traditional/more natural way of life (i.e. biological (organic) farming, natural food etc.) with a belief that “All natural things are good for life on the Earth”. In line with this trend, there is now an ever increasing lobby for using natural coloring matters for textile substrates both natural and synthetic [11,12]. The contemporary textile processing industry is getting more and more inquiries regarding “Dyeing with Natural Dyes” and therefore the subject of natural colors has assumed a great significance. Recently, an exhaustive review on the subject of natural dyes in textile applications has been published by Taylor .Acid dyes in general, are more resistant to ozone fading than disperse dyes and hence the latter almost entirely have been replaced by acid dyes in the nylon carpet dying industry .The poor resistance to ozone fading of disperse dyes has been attributed to their relatively small molecular size and lack of ionic character .Ozone is a strong oxidizing agent that destroys the chromophores of certain type of dyes. For example: ozone can attack the anthraquinone ring of a dye molecule and convert it into colorless phthalic acid derivatives .The outermost dry papery skins of Onion are the best source of the color, which contain flavonoid quercetol, kaempferol, quercetin-3-glucoside and some tannin. Lac is the resinous protective secretion of the tiny Lac insect, which is a pest on a number of plants. The insects secrete a thick resinous fluid, which envelops their bodies, forming a hard continuous encrustation over the twigs. The twigs are harvested and the encrustation scraped off dried and processed to yield shellac or the dye . Nylon is a polyamide that is mostly manufactured through condensation polymerization of di-amine and di-acid. Generally, nylon is dyed with acid dyes as well as reactive and disperse dyes [18, 19].Some researchers have studied dyeing nylon with natural dyes such as indigo, onion, lac, turmeric, kamala and henna [20, 18, and 8]. But the total share of natural dyes in the textile sector is approximately only 1 % due to certain technical and sustainability issues involved in the production and application of these dyes such as non-availability in ready-to-use standard form, unsuitability for machine use, and limited and non-reproducible shades. Natural dyes per se are sustainable as they are renewable and biodegradable but they cannot fulfill the huge demand from the textile sector in view of the preferential use of land for food and feed purposes.
2 Application of natural dyes on textiles Natural dyes are mostly employed for dyeing of natural fiber textiles to enhance their eco-friendly characteristics. They are usually applied to textiles by dyeing. Apart from indigo, other natural dyes are usually not used for printing directly. For producing printed fabrics, the printing is usually done with mordant and the whole material is dyed whereby only the area printed with mordant picks up the color. Natural dyes, like synthetic dyes, can also be used to dye textiles at all stages such as fiber, yarn, or fabric. Fiber dyeing has the advantage that any shade variation can be easily adjusted by blending and
International Journal of Scientific & Engineering Research, Volume 7, Issue 9, September-2016 1032 ISSN 2229-5518
IJSER © 2016 http://www.ijser.org
therefore has been practiced at industrial scale also but is costly due to problems in spinning and loss of dyed fibers. Wool is generally dyed in yarn form and traditional dyers prefer yarn dyeing for all materials as it offers versatility in designing during weaving. Dyeing is normally carried out by hand in large vessels. Iron, stainless steel, copper, and aluminum vessels are used. Dyeing in copper vessels is considered to produce bright shades. Aluminum vessels are normally stained with a particular dye hence should be used if only one type of dye is used. Stainless steel vessels are most preferred for the natural dyeing process. On a larger scale, hank-dyeing machines have been successfully used.
3 History of Nylon Fibers Nylon is a manufactured fiber in which the fiber forming substance is a long-chain synthetic polyamide in which less than 85% of the amide-linkages are attached directly (-CO-NH-) to two aliphatic groups. Nylon is a synthetic polymer, a plastic, invented on February 28, 1935 by Wallace Carothers at the E.I. du Pont de Nemours and Company of Wilmington, Delaware, USA. The material was announced in 1938 and the first nylon products; a nylon bristle toothbrush made with nylon yarn (went on sale on February 24, 1938) and more famously, women's stockings (went on sale on May 15, 1940). Nylon fibers are now used to make many synthetic fabrics, and solid nylon is used as an engineering material.
3.1 Characteristics of Nylon Fibers
• Exceptionally strong • Elastic • Abrasion resistant • Lustrous • Easy to wash • Resistant to damage from oil and many chemicals • Can be pre-colored or dyed in wide range of colors • Resilient • Low in moisture absorben